#------------------------------------------------------------------------------
#$Date: 2023-07-05 05:05:30 +0300 (Wed, 05 Jul 2023) $
#$Revision: 284807 $
#$URL: file:///home/coder/svn-repositories/cod/cif/2/31/21/2312138.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2312138
loop_
_publ_author_name
'Pavlyuk, Nazar'
'Dmytriv, Grygoriy'
'Pavlyuk, Volodymyr'
'Ciesielski, Wojciech'
'Rozdzynska-Kielbik, Beata'
'Indris, Sylvio'
'Ehrenberg, Helmut'
_publ_section_title
;
 A new ternary derivative of the Laves phases in the Mg-Co-Ga system.
;
_journal_issue                   4
_journal_name_full
'Acta crystallographica Section B, Structural science, crystal engineering and materials'
_journal_paper_doi               10.1107/S2052520623004511
_journal_volume                  79
_journal_year                    2023
_chemical_formula_moiety
'0.011(Ga8), 0.012(Ga8), 0.012(Ga8), 0.18(Ga0.20), 0.155(Ga), Co'
_chemical_formula_sum            'Co Ga0.52 Mg0.74'
_chemical_formula_weight         112.70
_space_group_crystal_system      orthorhombic
_space_group_IT_number           63
_space_group_name_Hall           '-C 2c 2'
_space_group_name_H-M_alt        'C m c m'
_audit_creation_method           SHELXL-2014/7
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            32
_cell_length_a                   4.9868(9)
_cell_length_b                   25.959(4)
_cell_length_c                   8.0508(11)
_cell_measurement_reflns_used    640
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      26.370
_cell_measurement_theta_min      2.977
_cell_volume                     1042.2(3)
_computing_cell_refinement       'CrysAlis CCD (Oxford Diffraction, 2008)'
_computing_data_collection       'CrysAlis CCD (Oxford Diffraction, 2008)'
_computing_data_reduction        'CrysAlis RED (Oxford Diffraction, 2008)'
_computing_molecular_graphics    'DIAMOND (Brandenburg, 2006)'
_computing_publication_material  'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_structure_solution    'SHELXS-2014/7 (Sheldrick, 2014)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.998
_diffrn_measured_fraction_theta_max 0.998
_diffrn_measurement_device_type  'Oxford Diffraction Xcalibur3 CCD'
_diffrn_measurement_method       'ω scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0925
_diffrn_reflns_av_unetI/netI     0.0587
_diffrn_reflns_Laue_measured_fraction_full 0.998
_diffrn_reflns_Laue_measured_fraction_max 0.998
_diffrn_reflns_limit_h_max       6
_diffrn_reflns_limit_h_min       -6
_diffrn_reflns_limit_k_max       32
_diffrn_reflns_limit_k_min       -32
_diffrn_reflns_limit_l_max       10
_diffrn_reflns_limit_l_min       -10
_diffrn_reflns_number            6142
_diffrn_reflns_point_group_measured_fraction_full 0.998
_diffrn_reflns_point_group_measured_fraction_max 0.998
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         26.370
_diffrn_reflns_theta_min         2.977
_diffrn_source                   'fine-focus sealed tube'
_exptl_absorpt_coefficient_mu    23.121
_exptl_absorpt_correction_T_max  0.630
_exptl_absorpt_correction_T_min  0.343
_exptl_absorpt_correction_type   analytical
_exptl_absorpt_process_details   '(CrysAlis RED; Oxford Diffraction, 2008)'
_exptl_crystal_colour            'metallic grey'
_exptl_crystal_density_diffrn    5.746
_exptl_crystal_density_meas      5.73(2)
_exptl_crystal_density_method    volumetric
_exptl_crystal_description       prism
_exptl_crystal_F_000             1657.1
_exptl_crystal_size_max          0.050
_exptl_crystal_size_mid          0.040
_exptl_crystal_size_min          0.020
_refine_diff_density_max         2.357
_refine_diff_density_min         -1.019
_refine_diff_density_rms         0.459
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   0.903
_refine_ls_matrix_type           full
_refine_ls_number_parameters     56
_refine_ls_number_reflns         640
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      0.903
_refine_ls_R_factor_all          0.0786
_refine_ls_R_factor_gt           0.0338
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0340P)²] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0622
_refine_ls_wR_factor_ref         0.0886
_reflns_Friedel_coverage         0.000
_reflns_number_gt                196
_reflns_number_total             640
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            ra5132sup1.cif
_cod_data_source_block           II-Mg0.74CoGa0.52
_cod_database_code               2312138
_shelx_shelxl_version_number     2014/7
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, z+1/2'
'x, -y, -z'
'-x, y, -z+1/2'
'x+1/2, y+1/2, z'
'-x+1/2, -y+1/2, z+1/2'
'x+1/2, -y+1/2, -z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x, y, -z-1/2'
'-x, y, z'
'x, -y, z-1/2'
'-x+1/2, -y+1/2, -z'
'x+1/2, y+1/2, -z-1/2'
'-x+1/2, y+1/2, z'
'x+1/2, -y+1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Co1 Co 0.0000 0.60972(10) 0.2500 0.0069(8) Uani 0.68 4 d S T P . .
Ga1 Ga 0.0000 0.60972(10) 0.2500 0.0069(8) Uani 0.32 4 d S T P . .
Co2 Co 0.0000 0.94270(11) 0.2500 0.0052(8) Uani 0.8 4 d S T P . .
Ga2 Ga 0.0000 0.94270(11) 0.2500 0.0052(8) Uani 0.2 4 d S T P . .
Co3 Co 0.0000 0.27584(11) 0.2500 0.0069(7) Uani 0.68 4 d S T P . .
Ga3 Ga 0.0000 0.27584(11) 0.2500 0.0069(7) Uani 0.32 4 d S T P . .
Co4 Co 0.0000 0.0000 0.0000 0.0062(7) Uani 0.68 4 d S T P . .
Ga4 Ga 0.0000 0.0000 0.0000 0.0062(7) Uani 0.32 4 d S T P . .
Co5 Co 0.0000 0.33331(8) -0.0006(2) 0.0074(4) Uani 0.7 2 d S T P . .
Ga5 Ga 0.0000 0.33331(8) -0.0006(2) 0.0074(4) Uani 0.3 2 d S T P . .
Co6 Co 0.2570(5) 0.02856(7) 0.2500 0.0072(5) Uani 0.64 2 d S T P . .
Ga6 Ga 0.2570(5) 0.02856(7) 0.2500 0.0072(5) Uani 0.36 2 d S T P . .
Co7 Co 0.2580(4) 0.36201(7) 0.2500 0.0075(6) Uani 0.62 2 d S T P . .
Ga7 Ga 0.2580(4) 0.36201(7) 0.2500 0.0075(6) Uani 0.38 2 d S T P . .
Co8 Co 0.2429(4) 0.19529(7) 0.2500 0.0074(5) Uani 0.62 2 d S T P . .
Ga8 Ga 0.2429(4) 0.19529(7) 0.2500 0.0074(5) Uani 0.38 2 d S T P . .
Mg1 Mg 0.0000 0.11103(16) 0.0649(8) 0.0043(13) Uani 1 2 d S T P . .
Mg2 Mg 0.0000 0.44471(17) 0.0654(7) 0.0066(13) Uani 1 2 d S T P . .
Mg Mg 0.0000 0.22209(17) 0.5662(6) 0.0095(11) Uiso 0.94 2 d S . P . .
Ga Ga 0.0000 0.22209(17) 0.5662(6) 0.0095(11) Uiso 0.06 2 d S . P . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Co Co 0.3494 0.9721 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ga Ga 0.2307 1.6083 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mg Mg 0.0486 0.0363 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
Ga6 Co1 Co6 0.0 5_455 5_455 ?
Ga6 Co1 Ga6 59.81(12) 5_455 15 ?
Co6 Co1 Ga6 59.81(12) 5_455 15 ?
Ga6 Co1 Co6 59.8 5_455 15 ?
Co6 Co1 Co6 59.81(12) 5_455 15 ?
Ga6 Co1 Co6 0.0 15 15 ?
Ga6 Co1 Ga5 120.94(5) 5_455 2_565 ?
Co6 Co1 Ga5 120.94(5) 5_455 2_565 ?
Ga6 Co1 Ga5 120.94(5) 15 2_565 ?
Co6 Co1 Ga5 120.94(5) 15 2_565 ?
Ga6 Co1 Co5 120.94(5) 5_455 2_565 ?
Co6 Co1 Co5 120.94(5) 5_455 2_565 ?
Ga6 Co1 Co5 120.94(5) 15 2_565 ?
Co6 Co1 Co5 120.94(5) 15 2_565 ?
Ga5 Co1 Co5 0.0 2_565 2_565 ?
Ga6 Co1 Ga5 120.94(5) 5_455 9_565 ?
Co6 Co1 Ga5 120.94(5) 5_455 9_565 ?
Ga6 Co1 Ga5 120.94(5) 15 9_565 ?
Co6 Co1 Ga5 120.94(5) 15 9_565 ?
Ga5 Co1 Ga5 107.25(14) 2_565 9_565 ?
Co5 Co1 Ga5 107.25(14) 2_565 9_565 ?
Ga6 Co1 Co5 120.94(5) 5_455 9_565 ?
Co6 Co1 Co5 120.94(5) 5_455 9_565 ?
Ga6 Co1 Co5 120.94(5) 15 9_565 ?
Co6 Co1 Co5 120.94(5) 15 9_565 ?
Ga5 Co1 Co5 107.2 2_565 9_565 ?
Co5 Co1 Co5 107.25(14) 2_565 9_565 ?
Ga5 Co1 Co5 0.0 9_565 9_565 ?
Ga6 Co1 Ga8 179.92(7) 5_455 15 ?
Co6 Co1 Ga8 179.92(7) 5_455 15 ?
Ga6 Co1 Ga8 120.11(8) 15 15 ?
Co6 Co1 Ga8 120.11(8) 15 15 ?
Ga5 Co1 Ga8 59.09(7) 2_565 15 ?
Co5 Co1 Ga8 59.09(7) 2_565 15 ?
Ga5 Co1 Ga8 59.09(7) 9_565 15 ?
Co5 Co1 Ga8 59.09(7) 9_565 15 ?
Ga6 Co1 Co8 179.92(7) 5_455 15 ?
Co6 Co1 Co8 179.92(7) 5_455 15 ?
Ga6 Co1 Co8 120.11(8) 15 15 ?
Co6 Co1 Co8 120.11(8) 15 15 ?
Ga5 Co1 Co8 59.09(7) 2_565 15 ?
Co5 Co1 Co8 59.09(7) 2_565 15 ?
Ga5 Co1 Co8 59.09(7) 9_565 15 ?
Co5 Co1 Co8 59.09(7) 9_565 15 ?
Ga8 Co1 Co8 0.0 15 15 ?
Ga6 Co1 Co8 120.11(8) 5_455 5_455 ?
Co6 Co1 Co8 120.11(8) 5_455 5_455 ?
Ga6 Co1 Co8 179.92(7) 15 5_455 ?
Co6 Co1 Co8 179.92(7) 15 5_455 ?
Ga5 Co1 Co8 59.09(7) 2_565 5_455 ?
Co5 Co1 Co8 59.09(7) 2_565 5_455 ?
Ga5 Co1 Co8 59.09(7) 9_565 5_455 ?
Co5 Co1 Co8 59.09(7) 9_565 5_455 ?
Ga8 Co1 Co8 60.0 15 5_455 ?
Co8 Co1 Co8 59.98(10) 15 5_455 ?
Ga6 Co1 Ga8 120.11(8) 5_455 5_455 ?
Co6 Co1 Ga8 120.11(8) 5_455 5_455 ?
Ga6 Co1 Ga8 179.92(7) 15 5_455 ?
Co6 Co1 Ga8 179.92(7) 15 5_455 ?
Ga5 Co1 Ga8 59.09(7) 2_565 5_455 ?
Co5 Co1 Ga8 59.09(7) 2_565 5_455 ?
Ga5 Co1 Ga8 59.09(7) 9_565 5_455 ?
Co5 Co1 Ga8 59.09(7) 9_565 5_455 ?
Ga8 Co1 Ga8 59.98(10) 15 5_455 ?
Co8 Co1 Ga8 59.98(10) 15 5_455 ?
Co8 Co1 Ga8 0.00(8) 5_455 5_455 ?
Ga7 Co2 Co7 0.0 5_455 5_455 ?
Ga7 Co2 Ga7 59.89(11) 5_455 15 ?
Co7 Co2 Ga7 59.89(11) 5_455 15 ?
Ga7 Co2 Co7 59.9 5_455 15 ?
Co7 Co2 Co7 59.89(11) 5_455 15 ?
Ga7 Co2 Co7 0.0 15 15 ?
Ga7 Co2 Ga4 121.00(4) 5_455 2_565 ?
Co7 Co2 Ga4 121.00(4) 5_455 2_565 ?
Ga7 Co2 Ga4 121.00(4) 15 2_565 ?
Co7 Co2 Ga4 121.00(4) 15 2_565 ?
Ga7 Co2 Co4 121.00(4) 5_455 2_565 ?
Co7 Co2 Co4 121.00(4) 5_455 2_565 ?
Ga7 Co2 Co4 121.00(4) 15 2_565 ?
Co7 Co2 Co4 121.00(4) 15 2_565 ?
Ga4 Co2 Co4 0.0 2_565 2_565 ?
Ga7 Co2 Ga4 121.00(4) 5_455 1_565 ?
Co7 Co2 Ga4 121.00(4) 5_455 1_565 ?
Ga7 Co2 Ga4 121.00(4) 15 1_565 ?
Co7 Co2 Ga4 121.00(4) 15 1_565 ?
Ga4 Co2 Ga4 107.06(10) 2_565 1_565 ?
Co4 Co2 Ga4 107.06(10) 2_565 1_565 ?
Ga7 Co2 Co4 121.00(4) 5_455 1_565 ?
Co7 Co2 Co4 121.00(4) 5_455 1_565 ?
Ga7 Co2 Co4 121.00(4) 15 1_565 ?
Co7 Co2 Co4 121.00(4) 15 1_565 ?
Ga4 Co2 Co4 107.1 2_565 1_565 ?
Co4 Co2 Co4 107.06(10) 2_565 1_565 ?
Ga4 Co2 Co4 0.0 1_565 1_565 ?
Ga7 Co2 Ga6 179.95(8) 5_455 1_565 ?
Co7 Co2 Ga6 179.95(8) 5_455 1_565 ?
Ga7 Co2 Ga6 120.15(8) 15 1_565 ?
Co7 Co2 Ga6 120.15(8) 15 1_565 ?
Ga4 Co2 Ga6 58.99(6) 2_565 1_565 ?
Co4 Co2 Ga6 58.99(6) 2_565 1_565 ?
Ga4 Co2 Ga6 58.99(6) 1_565 1_565 ?
Co4 Co2 Ga6 58.99(6) 1_565 1_565 ?
Ga7 Co2 Co6 179.95(8) 5_455 1_565 ?
Co7 Co2 Co6 179.95(8) 5_455 1_565 ?
Ga7 Co2 Co6 120.15(8) 15 1_565 ?
Co7 Co2 Co6 120.15(8) 15 1_565 ?
Ga4 Co2 Co6 58.99(6) 2_565 1_565 ?
Co4 Co2 Co6 58.99(6) 2_565 1_565 ?
Ga4 Co2 Co6 58.99(6) 1_565 1_565 ?
Co4 Co2 Co6 58.99(6) 1_565 1_565 ?
Ga6 Co2 Co6 0.0 1_565 1_565 ?
Ga7 Co2 Co6 120.15(8) 5_455 11_565 ?
Co7 Co2 Co6 120.15(8) 5_455 11_565 ?
Ga7 Co2 Co6 179.95(8) 15 11_565 ?
Co7 Co2 Co6 179.95(8) 15 11_565 ?
Ga4 Co2 Co6 58.99(6) 2_565 11_565 ?
Co4 Co2 Co6 58.99(6) 2_565 11_565 ?
Ga4 Co2 Co6 58.99(6) 1_565 11_565 ?
Co4 Co2 Co6 58.99(6) 1_565 11_565 ?
Ga6 Co2 Co6 59.8 1_565 11_565 ?
Co6 Co2 Co6 59.80(12) 1_565 11_565 ?
Ga7 Co2 Ga6 120.15(8) 5_455 11_565 ?
Co7 Co2 Ga6 120.15(8) 5_455 11_565 ?
Ga7 Co2 Ga6 179.95(8) 15 11_565 ?
Co7 Co2 Ga6 179.95(8) 15 11_565 ?
Ga4 Co2 Ga6 58.99(6) 2_565 11_565 ?
Co4 Co2 Ga6 58.99(6) 2_565 11_565 ?
Ga4 Co2 Ga6 58.99(6) 1_565 11_565 ?
Co4 Co2 Ga6 58.99(6) 1_565 11_565 ?
Ga6 Co2 Ga6 59.80(12) 1_565 11_565 ?
Co6 Co2 Ga6 59.80(12) 1_565 11_565 ?
Co6 Co2 Ga6 0.00(9) 11_565 11_565 ?
Co8 Co3 Ga8 60.2 . 11 ?
Co8 Co3 Co8 60.18(12) . 11 ?
Ga8 Co3 Co8 0.0 11 11 ?
Co8 Co3 Ga5 120.96(5) . 10_556 ?
Ga8 Co3 Ga5 120.96(5) 11 10_556 ?
Co8 Co3 Ga5 120.96(5) 11 10_556 ?
Co8 Co3 Co5 120.96(5) . 10_556 ?
Ga8 Co3 Co5 120.96(5) 11 10_556 ?
Co8 Co3 Co5 120.96(5) 11 10_556 ?
Ga5 Co3 Co5 0.0 10_556 10_556 ?
Co8 Co3 Co5 120.96(5) . . ?
Ga8 Co3 Co5 120.96(5) 11 . ?
Co8 Co3 Co5 120.96(5) 11 . ?
Ga5 Co3 Co5 107.0 10_556 . ?
Co5 Co3 Co5 107.04(15) 10_556 . ?
Co8 Co3 Co7 120.00(7) . . ?
Ga8 Co3 Co7 179.82(9) 11 . ?
Co8 Co3 Co7 179.82(9) 11 . ?
Ga5 Co3 Co7 58.98(7) 10_556 . ?
Co5 Co3 Co7 58.98(7) 10_556 . ?
Co5 Co3 Co7 58.98(7) . . ?
Co8 Co3 Ga7 179.82(9) . 11 ?
Ga8 Co3 Ga7 120.00(7) 11 11 ?
Co8 Co3 Ga7 120.00(7) 11 11 ?
Ga5 Co3 Ga7 58.98(7) 10_556 11 ?
Co5 Co3 Ga7 58.98(7) 10_556 11 ?
Co5 Co3 Ga7 58.98(7) . 11 ?
Co7 Co3 Ga7 59.8 . 11 ?
Co8 Co3 Co7 179.82(9) . 11 ?
Ga8 Co3 Co7 120.00(7) 11 11 ?
Co8 Co3 Co7 120.00(7) 11 11 ?
Ga5 Co3 Co7 58.98(7) 10_556 11 ?
Co5 Co3 Co7 58.98(7) 10_556 11 ?
Co5 Co3 Co7 58.98(7) . 11 ?
Co7 Co3 Co7 59.82(11) . 11 ?
Ga7 Co3 Co7 0.0 11 11 ?
Ga6 Co4 Co6 0.0 9 9 ?
Ga6 Co4 Ga6 118.28(9) 9 11 ?
Co6 Co4 Ga6 118.28(9) 9 11 ?
Ga6 Co4 Ga6 61.72(9) 9 3 ?
Co6 Co4 Ga6 61.72(9) 9 3 ?
Ga6 Co4 Ga6 180.00(13) 11 3 ?
Ga6 Co4 Co6 118.3 9 11 ?
Co6 Co4 Co6 118.28(9) 9 11 ?
Ga6 Co4 Co6 0.0 11 11 ?
Ga6 Co4 Co6 180.0 3 11 ?
Ga6 Co4 Co6 61.7 9 3 ?
Co6 Co4 Co6 61.72(9) 9 3 ?
Ga6 Co4 Co6 180.0 11 3 ?
Ga6 Co4 Co6 0.0 3 3 ?
Co6 Co4 Co6 180.00(13) 11 3 ?
Ga6 Co4 Co6 180.0 9 . ?
Co6 Co4 Co6 180.0 9 . ?
Ga6 Co4 Co6 61.7 11 . ?
Ga6 Co4 Co6 118.3 3 . ?
Co6 Co4 Co6 61.72(9) 11 . ?
Co6 Co4 Co6 118.28(9) 3 . ?
Ga6 Co4 Co2 118.13(6) 9 1_545 ?
Co6 Co4 Co2 118.13(6) 9 1_545 ?
Ga6 Co4 Co2 61.87(6) 11 1_545 ?
Ga6 Co4 Co2 118.13(6) 3 1_545 ?
Co6 Co4 Co2 61.87(6) 11 1_545 ?
Co6 Co4 Co2 118.13(6) 3 1_545 ?
Co6 Co4 Co2 61.87(6) . 1_545 ?
Ga6 Co4 Ga2 118.13(6) 9 1_545 ?
Co6 Co4 Ga2 118.13(6) 9 1_545 ?
Ga6 Co4 Ga2 61.87(6) 11 1_545 ?
Ga6 Co4 Ga2 118.13(6) 3 1_545 ?
Co6 Co4 Ga2 61.87(6) 11 1_545 ?
Co6 Co4 Ga2 118.13(6) 3 1_545 ?
Co6 Co4 Ga2 61.87(6) . 1_545 ?
Co2 Co4 Ga2 0.00(10) 1_545 1_545 ?
Ga6 Co4 Co2 61.87(6) 9 9_565 ?
Co6 Co4 Co2 61.87(6) 9 9_565 ?
Ga6 Co4 Co2 118.13(6) 11 9_565 ?
Ga6 Co4 Co2 61.87(6) 3 9_565 ?
Co6 Co4 Co2 118.13(6) 11 9_565 ?
Co6 Co4 Co2 61.87(6) 3 9_565 ?
Co6 Co4 Co2 118.13(6) . 9_565 ?
Co2 Co4 Co2 180.00(10) 1_545 9_565 ?
Ga2 Co4 Co2 180.0 1_545 9_565 ?
Ga6 Co4 Ga2 61.87(6) 9 9_565 ?
Co6 Co4 Ga2 61.87(6) 9 9_565 ?
Ga6 Co4 Ga2 118.13(6) 11 9_565 ?
Ga6 Co4 Ga2 61.87(6) 3 9_565 ?
Co6 Co4 Ga2 118.13(6) 11 9_565 ?
Co6 Co4 Ga2 61.87(6) 3 9_565 ?
Co6 Co4 Ga2 118.13(6) . 9_565 ?
Co2 Co4 Ga2 180.00(10) 1_545 9_565 ?
Ga2 Co4 Ga2 180.00(10) 1_545 9_565 ?
Co2 Co4 Ga2 0.00(10) 9_565 9_565 ?
Ga1 Co5 Co1 0.0 9_565 9_565 ?
Ga1 Co5 Ga8 61.88(7) 9_565 7_455 ?
Co1 Co5 Ga8 61.88(7) 9_565 7_455 ?
Ga1 Co5 Co8 61.88(7) 9_565 7_455 ?
Co1 Co5 Co8 61.88(7) 9_565 7_455 ?
Ga8 Co5 Co8 0.0 7_455 7_455 ?
Ga1 Co5 Ga8 61.88(7) 9_565 13 ?
Co1 Co5 Ga8 61.88(7) 9_565 13 ?
Ga8 Co5 Ga8 61.83(9) 7_455 13 ?
Co8 Co5 Ga8 61.83(9) 7_455 13 ?
Ga1 Co5 Co8 61.88(7) 9_565 13 ?
Co1 Co5 Co8 61.88(7) 9_565 13 ?
Ga8 Co5 Co8 61.8 7_455 13 ?
Co8 Co5 Co8 61.83(9) 7_455 13 ?
Ga8 Co5 Co8 0.0 13 13 ?
Ga1 Co5 Co7 118.16(10) 9_565 . ?
Co1 Co5 Co7 118.16(10) 9_565 . ?
Ga8 Co5 Co7 179.97(13) 7_455 . ?
Co8 Co5 Co7 179.97(13) 7_455 . ?
Ga8 Co5 Co7 118.19(5) 13 . ?
Co8 Co5 Co7 118.19(5) 13 . ?
Ga1 Co5 Co7 118.16(10) 9_565 11 ?
Co1 Co5 Co7 118.16(10) 9_565 11 ?
Ga8 Co5 Co7 118.19(5) 7_455 11 ?
Co8 Co5 Co7 118.19(5) 7_455 11 ?
Ga8 Co5 Co7 179.97(13) 13 11 ?
Co8 Co5 Co7 179.97(13) 13 11 ?
Co7 Co5 Co7 61.78(8) . 11 ?
Ga1 Co5 Ga7 118.16(10) 9_565 11 ?
Co1 Co5 Ga7 118.16(10) 9_565 11 ?
Ga8 Co5 Ga7 118.19(5) 7_455 11 ?
Co8 Co5 Ga7 118.19(5) 7_455 11 ?
Ga8 Co5 Ga7 179.97(13) 13 11 ?
Co8 Co5 Ga7 179.97(13) 13 11 ?
Co7 Co5 Ga7 61.8 . 11 ?
Co7 Co5 Ga7 0.00(11) 11 11 ?
Ga1 Co5 Co3 179.89(13) 9_565 . ?
Co1 Co5 Co3 179.89(13) 9_565 . ?
Ga8 Co5 Co3 118.04(9) 7_455 . ?
Co8 Co5 Co3 118.04(9) 7_455 . ?
Ga8 Co5 Co3 118.04(9) 13 . ?
Co8 Co5 Co3 118.04(9) 13 . ?
Co7 Co5 Co3 61.93(6) . . ?
Co7 Co5 Co3 61.93(6) 11 . ?
Ga7 Co5 Co3 61.93(6) 11 . ?
Ga6 Co6 Co6 0.0 11_655 11_655 ?
Ga6 Co6 Ga1 60.10(6) 11_655 5_545 ?
Co6 Co6 Ga1 60.10(6) 11_655 5_545 ?
Ga6 Co6 Co1 60.10(6) 11_655 5_545 ?
Co6 Co6 Co1 60.10(6) 11_655 5_545 ?
Ga1 Co6 Co1 0.0 5_545 5_545 ?
Ga6 Co6 Co4 120.86(5) 11_655 . ?
Co6 Co6 Co4 120.86(5) 11_655 . ?
Ga1 Co6 Co4 120.86(4) 5_545 . ?
Co1 Co6 Co4 120.86(4) 5_545 . ?
Ga6 Co6 Ga4 120.86(5) 11_655 2 ?
Co6 Co6 Ga4 120.86(5) 11_655 2 ?
Ga1 Co6 Ga4 120.86(4) 5_545 2 ?
Co1 Co6 Ga4 120.86(4) 5_545 2 ?
Co4 Co6 Ga4 107.3 . 2 ?
Ga6 Co6 Co4 120.86(5) 11_655 2 ?
Co6 Co6 Co4 120.86(5) 11_655 2 ?
Ga1 Co6 Co4 120.86(4) 5_545 2 ?
Co1 Co6 Co4 120.86(4) 5_545 2 ?
Co4 Co6 Co4 107.32(9) . 2 ?
Ga4 Co6 Co4 0.0 2 2 ?
Ga6 Co6 Ga6 180.0 11_655 11 ?
Co6 Co6 Ga6 180.0 11_655 11 ?
Ga1 Co6 Ga6 119.91(6) 5_545 11 ?
Co1 Co6 Ga6 119.91(6) 5_545 11 ?
Co4 Co6 Ga6 59.14(5) . 11 ?
Ga4 Co6 Ga6 59.14(5) 2 11 ?
Co4 Co6 Ga6 59.14(5) 2 11 ?
Ga6 Co6 Co6 180.0 11_655 11 ?
Co6 Co6 Co6 180.0 11_655 11 ?
Ga1 Co6 Co6 119.91(6) 5_545 11 ?
Co1 Co6 Co6 119.91(6) 5_545 11 ?
Co4 Co6 Co6 59.14(5) . 11 ?
Ga4 Co6 Co6 59.14(5) 2 11 ?
Co4 Co6 Co6 59.14(5) 2 11 ?
Ga6 Co6 Co6 0.0 11 11 ?
Ga6 Co6 Ga2 119.90(6) 11_655 1_545 ?
Co6 Co6 Ga2 119.90(6) 11_655 1_545 ?
Ga1 Co6 Ga2 179.99(11) 5_545 1_545 ?
Co1 Co6 Ga2 179.99(11) 5_545 1_545 ?
Co4 Co6 Ga2 59.14(5) . 1_545 ?
Ga4 Co6 Ga2 59.14(5) 2 1_545 ?
Co4 Co6 Ga2 59.14(5) 2 1_545 ?
Ga6 Co6 Ga2 60.10(6) 11 1_545 ?
Co6 Co6 Ga2 60.10(6) 11 1_545 ?
Ga6 Co6 Co2 119.90(6) 11_655 1_545 ?
Co6 Co6 Co2 119.90(6) 11_655 1_545 ?
Ga1 Co6 Co2 179.99(11) 5_545 1_545 ?
Co1 Co6 Co2 179.99(11) 5_545 1_545 ?
Co4 Co6 Co2 59.14(5) . 1_545 ?
Ga4 Co6 Co2 59.14(5) 2 1_545 ?
Co4 Co6 Co2 59.14(5) 2 1_545 ?
Ga6 Co6 Co2 60.10(6) 11 1_545 ?
Co6 Co6 Co2 60.10(6) 11 1_545 ?
Ga2 Co6 Co2 0.0 1_545 1_545 ?
Ga7 Co7 Co7 0.0 11_655 11_655 ?
Ga7 Co7 Ga2 60.05(5) 11_655 5_545 ?
Co7 Co7 Ga2 60.05(5) 11_655 5_545 ?
Ga7 Co7 Co2 60.05(5) 11_655 5_545 ?
Co7 Co7 Co2 60.05(5) 11_655 5_545 ?
Ga2 Co7 Co2 0.0 5_545 5_545 ?
Ga7 Co7 Ga5 120.89(4) 11_655 10_556 ?
Co7 Co7 Ga5 120.89(4) 11_655 10_556 ?
Ga2 Co7 Ga5 120.92(6) 5_545 10_556 ?
Co2 Co7 Ga5 120.92(6) 5_545 10_556 ?
Ga7 Co7 Co5 120.89(4) 11_655 10_556 ?
Co7 Co7 Co5 120.89(4) 11_655 10_556 ?
Ga2 Co7 Co5 120.92(6) 5_545 10_556 ?
Co2 Co7 Co5 120.92(6) 5_545 10_556 ?
Ga5 Co7 Co5 0.0 10_556 10_556 ?
Ga7 Co7 Co5 120.89(4) 11_655 . ?
Co7 Co7 Co5 120.89(4) 11_655 . ?
Ga2 Co7 Co5 120.92(6) 5_545 . ?
Co2 Co7 Co5 120.92(6) 5_545 . ?
Ga5 Co7 Co5 107.2 10_556 . ?
Co5 Co7 Co5 107.22(10) 10_556 . ?
Ga7 Co7 Ga7 180.0 11_655 11 ?
Co7 Co7 Ga7 180.0 11_655 11 ?
Ga2 Co7 Ga7 119.94(5) 5_545 11 ?
Co2 Co7 Ga7 119.94(5) 5_545 11 ?
Ga5 Co7 Ga7 59.11(4) 10_556 11 ?
Co5 Co7 Ga7 59.11(4) 10_556 11 ?
Co5 Co7 Ga7 59.11(4) . 11 ?
Ga7 Co7 Co7 180.0 11_655 11 ?
Co7 Co7 Co7 180.0 11_655 11 ?
Ga2 Co7 Co7 119.94(5) 5_545 11 ?
Co2 Co7 Co7 119.94(5) 5_545 11 ?
Ga5 Co7 Co7 59.11(4) 10_556 11 ?
Co5 Co7 Co7 59.11(4) 10_556 11 ?
Co5 Co7 Co7 59.11(4) . 11 ?
Ga7 Co7 Co7 0.0 11 11 ?
Ga7 Co7 Co3 119.91(6) 11_655 . ?
Co7 Co7 Co3 119.91(6) 11_655 . ?
Ga2 Co7 Co3 179.96(9) 5_545 . ?
Co2 Co7 Co3 179.96(9) 5_545 . ?
Ga5 Co7 Co3 59.09(6) 10_556 . ?
Co5 Co7 Co3 59.09(6) 10_556 . ?
Co5 Co7 Co3 59.09(6) . . ?
Ga7 Co7 Co3 60.09(6) 11 . ?
Co7 Co7 Co3 60.09(6) 11 . ?
Co3 Co8 Ga8 59.91(6) . 11 ?
Co3 Co8 Co8 59.91(6) . 11 ?
Ga8 Co8 Co8 0.0 11 11 ?
Co3 Co8 Ga5 121.00(7) . 6 ?
Ga8 Co8 Ga5 120.91(4) 11 6 ?
Co8 Co8 Ga5 120.91(4) 11 6 ?
Co3 Co8 Co5 121.00(7) . 6 ?
Ga8 Co8 Co5 120.91(4) 11 6 ?
Co8 Co8 Co5 120.91(4) 11 6 ?
Ga5 Co8 Co5 0.0 6 6 ?
Co3 Co8 Ga5 121.00(7) . 13 ?
Ga8 Co8 Ga5 120.91(4) 11 13 ?
Co8 Co8 Ga5 120.91(4) 11 13 ?
Ga5 Co8 Ga5 107.15(9) 6 13 ?
Co5 Co8 Ga5 107.15(9) 6 13 ?
Co3 Co8 Co5 121.00(7) . 13 ?
Ga8 Co8 Co5 120.91(4) 11 13 ?
Co8 Co8 Co5 120.91(4) 11 13 ?
Ga5 Co8 Co5 107.2 6 13 ?
Co5 Co8 Co5 107.15(9) 6 13 ?
Ga5 Co8 Co5 0.0 13 13 ?
Co3 Co8 Ga8 120.09(6) . 11_655 ?
Ga8 Co8 Ga8 180.0 11 11_655 ?
Co8 Co8 Ga8 180.0 11 11_655 ?
Ga5 Co8 Ga8 59.08(4) 6 11_655 ?
Co5 Co8 Ga8 59.08(4) 6 11_655 ?
Ga5 Co8 Ga8 59.08(4) 13 11_655 ?
Co5 Co8 Ga8 59.08(4) 13 11_655 ?
Co3 Co8 Co8 120.09(6) . 11_655 ?
Ga8 Co8 Co8 180.0 11 11_655 ?
Co8 Co8 Co8 180.0 11 11_655 ?
Ga5 Co8 Co8 59.08(4) 6 11_655 ?
Co5 Co8 Co8 59.08(4) 6 11_655 ?
Ga5 Co8 Co8 59.08(4) 13 11_655 ?
Co5 Co8 Co8 59.08(4) 13 11_655 ?
Ga8 Co8 Co8 0.0 11_655 11_655 ?
Co3 Co8 Co1 179.90(10) . 5_545 ?
Ga8 Co8 Co1 119.99(5) 11 5_545 ?
Co8 Co8 Co1 119.99(5) 11 5_545 ?
Ga5 Co8 Co1 59.03(6) 6 5_545 ?
Co5 Co8 Co1 59.03(6) 6 5_545 ?
Ga5 Co8 Co1 59.03(6) 13 5_545 ?
Co5 Co8 Co1 59.03(6) 13 5_545 ?
Ga8 Co8 Co1 60.01(5) 11_655 5_545 ?
Co8 Co8 Co1 60.01(5) 11_655 5_545 ?
Co3 Co8 Ga1 179.90(10) . 5_545 ?
Ga8 Co8 Ga1 119.99(5) 11 5_545 ?
Co8 Co8 Ga1 119.99(5) 11 5_545 ?
Ga5 Co8 Ga1 59.03(6) 6 5_545 ?
Co5 Co8 Ga1 59.03(6) 6 5_545 ?
Ga5 Co8 Ga1 59.03(6) 13 5_545 ?
Co5 Co8 Ga1 59.03(6) 13 5_545 ?
Ga8 Co8 Ga1 60.01(5) 11_655 5_545 ?
Co8 Co8 Ga1 60.01(5) 11_655 5_545 ?
Co1 Co8 Ga1 0.00(6) 5_545 5_545 ?
Ga2 Mg1 Co2 0.0 9_565 9_565 ?
Ga2 Mg1 Ga7 49.37(11) 9_565 7_455 ?
Co2 Mg1 Ga7 49.37(11) 9_565 7_455 ?
Ga2 Mg1 Co7 49.37(11) 9_565 7_455 ?
Co2 Mg1 Co7 49.37(11) 9_565 7_455 ?
Ga7 Mg1 Co7 0.0 7_455 7_455 ?
Ga2 Mg1 Ga7 49.37(11) 9_565 13 ?
Co2 Mg1 Ga7 49.37(11) 9_565 13 ?
Ga7 Mg1 Ga7 49.28(12) 7_455 13 ?
Co7 Mg1 Ga7 49.28(12) 7_455 13 ?
Ga2 Mg1 Co7 49.37(11) 9_565 13 ?
Co2 Mg1 Co7 49.37(11) 9_565 13 ?
Ga7 Mg1 Co7 49.3 7_455 13 ?
Co7 Mg1 Co7 49.28(12) 7_455 13 ?
Ga7 Mg1 Co7 0.0 13 13 ?
Ga2 Mg1 Ga1 116.34(11) 9_565 5_545 ?
Co2 Mg1 Ga1 116.34(11) 9_565 5_545 ?
Ga7 Mg1 Ga1 144.11(16) 7_455 5_545 ?
Co7 Mg1 Ga1 144.11(16) 7_455 5_545 ?
Ga7 Mg1 Ga1 95.41(7) 13 5_545 ?
Co7 Mg1 Ga1 95.41(7) 13 5_545 ?
Ga2 Mg1 Co1 116.34(11) 9_565 5_545 ?
Co2 Mg1 Co1 116.34(11) 9_565 5_545 ?
Ga7 Mg1 Co1 144.11(16) 7_455 5_545 ?
Co7 Mg1 Co1 144.11(16) 7_455 5_545 ?
Ga7 Mg1 Co1 95.41(7) 13 5_545 ?
Co7 Mg1 Co1 95.41(7) 13 5_545 ?
Ga1 Mg1 Co1 0.0 5_545 5_545 ?
Ga2 Mg1 Co1 116.34(11) 9_565 5_445 ?
Co2 Mg1 Co1 116.34(11) 9_565 5_445 ?
Ga7 Mg1 Co1 95.41(7) 7_455 5_445 ?
Co7 Mg1 Co1 95.41(7) 7_455 5_445 ?
Ga7 Mg1 Co1 144.11(16) 13 5_445 ?
Co7 Mg1 Co1 144.11(16) 13 5_445 ?
Ga1 Mg1 Co1 118.3 5_545 5_445 ?
Co1 Mg1 Co1 118.3(2) 5_545 5_445 ?
Ga2 Mg1 Ga1 116.34(11) 9_565 5_445 ?
Co2 Mg1 Ga1 116.34(11) 9_565 5_445 ?
Ga7 Mg1 Ga1 95.41(7) 7_455 5_445 ?
Co7 Mg1 Ga1 95.41(7) 7_455 5_445 ?
Ga7 Mg1 Ga1 144.11(16) 13 5_445 ?
Co7 Mg1 Ga1 144.11(16) 13 5_445 ?
Ga1 Mg1 Ga1 118.3(2) 5_545 5_445 ?
Co1 Mg1 Ga1 118.3(2) 5_545 5_445 ?
Co1 Mg1 Ga1 0.00(10) 5_445 5_445 ?
Ga2 Mg1 Co6 95.40(14) 9_565 . ?
Co2 Mg1 Co6 95.40(14) 9_565 . ?
Ga7 Mg1 Co6 144.2(2) 7_455 . ?
Co7 Mg1 Co6 144.2(2) 7_455 . ?
Ga7 Mg1 Co6 116.32(12) 13 . ?
Co7 Mg1 Co6 116.32(12) 13 . ?
Ga1 Mg1 Co6 49.45(9) 5_545 . ?
Co1 Mg1 Co6 49.45(9) 5_545 . ?
Co1 Mg1 Co6 96.14(17) 5_445 . ?
Ga1 Mg1 Co6 96.14(17) 5_445 . ?
Ga6 Mg2 Co6 0.0 7_455 7_455 ?
Ga6 Mg2 Ga6 49.44(12) 7_455 13 ?
Co6 Mg2 Ga6 49.44(12) 7_455 13 ?
Ga6 Mg2 Co6 49.4 7_455 13 ?
Co6 Mg2 Co6 49.44(12) 7_455 13 ?
Ga6 Mg2 Co6 0.0 13 13 ?
Ga6 Mg2 Ga6 116.35(15) 7_455 15 ?
Co6 Mg2 Ga6 116.35(15) 7_455 15 ?
Ga6 Mg2 Ga6 95.42(11) 13 15 ?
Co6 Mg2 Ga6 95.42(11) 13 15 ?
Ga6 Mg2 Co6 116.4 7_455 15 ?
Co6 Mg2 Co6 116.35(15) 7_455 15 ?
Ga6 Mg2 Co6 95.4 13 15 ?
Co6 Mg2 Co6 95.42(11) 13 15 ?
Ga6 Mg2 Co6 0.0 15 15 ?
Ga6 Mg2 Ga6 95.42(11) 7_455 5_455 ?
Co6 Mg2 Ga6 95.42(11) 7_455 5_455 ?
Ga6 Mg2 Ga6 116.35(15) 13 5_455 ?
Co6 Mg2 Ga6 116.35(15) 13 5_455 ?
Ga6 Mg2 Ga6 49.38(13) 15 5_455 ?
Co6 Mg2 Ga6 49.38(13) 15 5_455 ?
Ga6 Mg2 Co6 95.4 7_455 5_455 ?
Co6 Mg2 Co6 95.42(11) 7_455 5_455 ?
Ga6 Mg2 Co6 116.4 13 5_455 ?
Co6 Mg2 Co6 116.35(15) 13 5_455 ?
Ga6 Mg2 Co6 49.4 15 5_455 ?
Co6 Mg2 Co6 49.38(13) 15 5_455 ?
Ga6 Mg2 Co6 0.0 5_455 5_455 ?
Ga6 Mg2 Co2 144.29(14) 7_455 5_545 ?
Co6 Mg2 Co2 144.29(14) 7_455 5_545 ?
Ga6 Mg2 Co2 95.38(7) 13 5_545 ?
Co6 Mg2 Co2 95.38(7) 13 5_545 ?
Ga6 Mg2 Co2 52.59(9) 15 5_545 ?
Co6 Mg2 Co2 52.59(9) 15 5_545 ?
Ga6 Mg2 Co2 96.31(16) 5_455 5_545 ?
Co6 Mg2 Co2 96.31(16) 5_455 5_545 ?
Ga6 Mg2 Ga2 144.29(14) 7_455 5_545 ?
Co6 Mg2 Ga2 144.29(14) 7_455 5_545 ?
Ga6 Mg2 Ga2 95.38(7) 13 5_545 ?
Co6 Mg2 Ga2 95.38(7) 13 5_545 ?
Ga6 Mg2 Ga2 52.59(9) 15 5_545 ?
Co6 Mg2 Ga2 52.59(9) 15 5_545 ?
Ga6 Mg2 Ga2 96.31(16) 5_455 5_545 ?
Co6 Mg2 Ga2 96.31(16) 5_455 5_545 ?
Co2 Mg2 Ga2 0.00(11) 5_545 5_545 ?
Ga6 Mg2 Co2 95.38(7) 7_455 5_445 ?
Co6 Mg2 Co2 95.38(7) 7_455 5_445 ?
Ga6 Mg2 Co2 144.29(14) 13 5_445 ?
Co6 Mg2 Co2 144.29(14) 13 5_445 ?
Ga6 Mg2 Co2 96.31(16) 15 5_445 ?
Co6 Mg2 Co2 96.31(16) 15 5_445 ?
Ga6 Mg2 Co2 52.59(9) 5_455 5_445 ?
Co6 Mg2 Co2 52.59(9) 5_455 5_445 ?
Co2 Mg2 Co2 118.37(18) 5_545 5_445 ?
Ga2 Mg2 Co2 118.4 5_545 5_445 ?
Ga6 Mg2 Ga2 95.38(7) 7_455 5_445 ?
Co6 Mg2 Ga2 95.38(7) 7_455 5_445 ?
Ga6 Mg2 Ga2 144.29(14) 13 5_445 ?
Co6 Mg2 Ga2 144.29(14) 13 5_445 ?
Ga6 Mg2 Ga2 96.31(16) 15 5_445 ?
Co6 Mg2 Ga2 96.31(16) 15 5_445 ?
Ga6 Mg2 Ga2 52.59(9) 5_455 5_445 ?
Co6 Mg2 Ga2 52.59(9) 5_455 5_445 ?
Co2 Mg2 Ga2 118.37(18) 5_545 5_445 ?
Ga2 Mg2 Ga2 118.37(18) 5_545 5_445 ?
Co2 Mg2 Ga2 0.00(11) 5_445 5_445 ?
Ga3 Mg Co3 0.0 13_556 13_556 ?
Ga3 Mg Ga3 118.58(18) 13_556 13_456 ?
Co3 Mg Ga3 118.58(18) 13_556 13_456 ?
Ga3 Mg Co3 118.6 13_556 13_456 ?
Co3 Mg Co3 118.58(18) 13_556 13_456 ?
Ga3 Mg Co3 0.0 13_456 13_456 ?
Ga3 Mg Ga7 96.38(15) 13_556 7_456 ?
Co3 Mg Ga7 96.38(15) 13_556 7_456 ?
Ga3 Mg Ga7 52.83(8) 13_456 7_456 ?
Co3 Mg Ga7 52.83(8) 13_456 7_456 ?
Ga3 Mg Co7 96.38(15) 13_556 7_456 ?
Co3 Mg Co7 96.38(15) 13_556 7_456 ?
Ga3 Mg Co7 52.83(8) 13_456 7_456 ?
Co3 Mg Co7 52.83(8) 13_456 7_456 ?
Ga7 Mg Co7 0.0 7_456 7_456 ?
Ga3 Mg Ga7 52.83(8) 13_556 13_556 ?
Co3 Mg Ga7 52.83(8) 13_556 13_556 ?
Ga3 Mg Ga7 96.38(15) 13_456 13_556 ?
Co3 Mg Ga7 96.38(15) 13_456 13_556 ?
Ga7 Mg Ga7 49.16(11) 7_456 13_556 ?
Co7 Mg Ga7 49.16(11) 7_456 13_556 ?
Ga3 Mg Co7 52.83(8) 13_556 13_556 ?
Co3 Mg Co7 52.83(8) 13_556 13_556 ?
Ga3 Mg Co7 96.38(15) 13_456 13_556 ?
Co3 Mg Co7 96.38(15) 13_456 13_556 ?
Ga7 Mg Co7 49.2 7_456 13_556 ?
Co7 Mg Co7 49.16(11) 7_456 13_556 ?
Ga7 Mg Co7 0.0 13_556 13_556 ?
Ga3 Mg Co3 116.0 13_556 . ?
Co3 Mg Co3 116.02(9) 13_556 . ?
Ga3 Mg Co3 116.0 13_456 . ?
Co3 Mg Co3 116.02(9) 13_456 . ?
Ga7 Mg Co3 144.03(14) 7_456 . ?
Co7 Mg Co3 144.03(14) 7_456 . ?
Ga7 Mg Co3 144.03(14) 13_556 . ?
Co7 Mg Co3 144.03(14) 13_556 . ?
Ga3 Mg Co8 95.34(6) 13_556 . ?
Co3 Mg Co8 95.34(6) 13_556 . ?
Ga3 Mg Co8 144.15(14) 13_456 . ?
Co3 Mg Co8 144.15(14) 13_456 . ?
Ga7 Mg Co8 116.14(16) 7_456 . ?
Co7 Mg Co8 116.14(16) 7_456 . ?
Ga7 Mg Co8 95.36(11) 13_556 . ?
Co7 Mg Co8 95.36(11) 13_556 . ?
Co3 Mg Co8 49.19(9) . . ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Co1 Ga6 2.430(3) 5_455 ?
Co1 Co6 2.430(3) 5_455 ?
Co1 Ga6 2.430(3) 15 ?
Co1 Co6 2.430(3) 15 ?
Co1 Ga5 2.494(3) 2_565 ?
Co1 Co5 2.494(3) 2_565 ?
Co1 Ga5 2.494(3) 9_565 ?
Co1 Co5 2.494(3) 9_565 ?
Co1 Ga8 2.565(3) 15 ?
Co1 Co8 2.565(3) 15 ?
Co1 Co8 2.565(3) 5_455 ?
Co1 Ga8 2.565(3) 5_455 ?
Co2 Ga7 2.417(3) 5_455 ?
Co2 Co7 2.417(3) 5_455 ?
Co2 Ga7 2.417(3) 15 ?
Co2 Co7 2.417(3) 15 ?
Co2 Ga4 2.5028(17) 2_565 ?
Co2 Co4 2.5028(17) 2_565 ?
Co2 Ga4 2.5028(17) 1_565 ?
Co2 Co4 2.5028(17) 1_565 ?
Co2 Ga6 2.571(3) 1_565 ?
Co2 Co6 2.571(3) 1_565 ?
Co2 Co6 2.571(3) 11_565 ?
Co2 Ga6 2.571(3) 11_565 ?
Co3 Co8 2.417(3) . ?
Co3 Ga8 2.417(3) 11 ?
Co3 Co8 2.417(3) 11 ?
Co3 Ga5 2.509(3) 10_556 ?
Co3 Co5 2.509(3) 10_556 ?
Co3 Co5 2.509(3) . ?
Co3 Co7 2.581(3) . ?
Co3 Ga7 2.581(3) 11 ?
Co3 Co7 2.581(3) 11 ?
Co4 Ga6 2.4986(14) 9 ?
Co4 Co6 2.4986(14) 9 ?
Co4 Ga6 2.4986(14) 11 ?
Co4 Ga6 2.4986(14) 3 ?
Co4 Co6 2.4986(14) 11 ?
Co4 Co6 2.4986(14) 3 ?
Co4 Co6 2.4986(14) . ?
Co4 Co2 2.5028(17) 1_545 ?
Co4 Ga2 2.5028(17) 1_545 ?
Co4 Co2 2.5028(17) 9_565 ?
Co4 Ga2 2.5028(17) 9_565 ?
Co5 Ga1 2.494(3) 9_565 ?
Co5 Co1 2.494(3) 9_565 ?
Co5 Ga8 2.495(2) 7_455 ?
Co5 Co8 2.495(2) 7_455 ?
Co5 Ga8 2.495(2) 13 ?
Co5 Co8 2.495(2) 13 ?
Co5 Co7 2.506(2) . ?
Co5 Co7 2.506(2) 11 ?
Co5 Ga7 2.506(2) 11 ?
Co6 Ga6 2.424(5) 11_655 ?
Co6 Co6 2.424(5) 11_655 ?
Co6 Ga1 2.430(3) 5_545 ?
Co6 Co1 2.430(3) 5_545 ?
Co6 Ga4 2.4986(14) 2 ?
Co6 Co4 2.4986(14) 2 ?
Co6 Ga6 2.563(5) 11 ?
Co6 Co6 2.563(5) 11 ?
Co6 Ga2 2.571(3) 1_545 ?
Co6 Co2 2.571(3) 1_545 ?
Co7 Ga7 2.413(4) 11_655 ?
Co7 Co7 2.413(4) 11_655 ?
Co7 Ga2 2.417(3) 5_545 ?
Co7 Co2 2.417(3) 5_545 ?
Co7 Ga5 2.506(2) 10_556 ?
Co7 Co5 2.506(2) 10_556 ?
Co7 Ga7 2.574(4) 11 ?
Co7 Co7 2.574(4) 11 ?
Co8 Ga8 2.423(4) 11 ?
Co8 Co8 2.423(4) 11 ?
Co8 Ga5 2.495(2) 6 ?
Co8 Co5 2.495(2) 6 ?
Co8 Ga5 2.495(2) 13 ?
Co8 Co5 2.495(2) 13 ?
Co8 Ga8 2.564(4) 11_655 ?
Co8 Co8 2.564(4) 11_655 ?
Co8 Co1 2.565(3) 5_545 ?
Co8 Ga1 2.565(3) 5_545 ?
Mg1 Ga2 2.894(6) 9_565 ?
Mg1 Co2 2.894(6) 9_565 ?
Mg1 Ga7 2.894(6) 7_455 ?
Mg1 Co7 2.894(6) 7_455 ?
Mg1 Ga7 2.894(6) 13 ?
Mg1 Co7 2.894(6) 13 ?
Mg1 Ga1 2.905(3) 5_545 ?
Mg1 Co1 2.905(3) 5_545 ?
Mg1 Co1 2.905(3) 5_445 ?
Mg1 Ga1 2.905(3) 5_445 ?
Mg2 Ga6 2.898(5) 7_455 ?
Mg2 Co6 2.898(5) 7_455 ?
Mg2 Ga6 2.898(5) 13 ?
Mg2 Co6 2.898(5) 13 ?
Mg2 Ga6 2.901(5) 15 ?
Mg2 Co6 2.901(5) 15 ?
Mg2 Ga6 2.901(5) 5_455 ?
Mg2 Co6 2.901(5) 5_455 ?
Mg2 Co2 2.903(3) 5_545 ?
Mg2 Ga2 2.903(3) 5_545 ?
Mg2 Co2 2.903(3) 5_445 ?
Mg2 Ga2 2.903(3) 5_445 ?
Mg Ga3 2.900(3) 13_556 ?
Mg Co3 2.900(3) 13_556 ?
Mg Ga3 2.900(3) 13_456 ?
Mg Co3 2.900(3) 13_456 ?
Mg Ga7 2.901(5) 7_456 ?
Mg Co7 2.901(5) 7_456 ?
Mg Ga7 2.901(5) 13_556 ?
Mg Co7 2.901(5) 13_556 ?

_cod_database_fobs_code 2312138
